#------------------------------------------------------------------------------
#$Date: 2016-03-22 23:43:21 +0200 (Tue, 22 Mar 2016) $
#$Revision: 179074 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/36/4303670.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4303670
loop_
_publ_author_name
'Asako Igashira-Kamiyama'
'Takashi Kajiwara'
'Motohiro Nakano'
'Takumi Konno'
'Tasuku Ito'
_publ_contact_author_address
; Department of Chemistry, Graduate School of Science,
  Osaka University, Toyonaka 560-0043, JAPAN
;
_publ_contact_author_email       ' igashira@chem.sci.osaka-u.ac.jp '
_publ_contact_author_fax         ' 81-6-6850-5765 '
_publ_contact_author_name        'Asako Igashira-Kamiyama'
_publ_contact_author_phone       ' 81-6-6850-5786 '
_publ_section_title
;
Syntheses, Structures, and Magnetic Properties of Tetramanganese(III) and
Hexamanganese(III) Complexes Containing Derivative of Biguanidate Ligand:
Ferromagnetic Interaction via Imino Nitrogen
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11388
_journal_page_last               11393
_journal_paper_doi               10.1021/ic901219f
_journal_volume                  48
_journal_year                    2009
_chemical_formula_sum            'C32 H62 Mn6 N24 O20'
_chemical_formula_weight         1432.70
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 108.533(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   12.348(2)
_cell_length_b                   24.911(5)
_cell_length_c                   9.7567(18)
_cell_measurement_reflns_used    788
_cell_measurement_temperature    223(2)
_cell_measurement_theta_max      27.61
_cell_measurement_theta_min      1.63
_cell_volume                     2845.5(9)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      223(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0835
_diffrn_reflns_av_sigmaI/netI    0.1191
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            13793
_diffrn_reflns_theta_full        27.61
_diffrn_reflns_theta_max         27.61
_diffrn_reflns_theta_min         1.63
_exptl_absorpt_coefficient_mu    1.381
_exptl_absorpt_correction_T_max  0.862075
_exptl_absorpt_correction_T_min  0.761301
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            'dark orange'
_exptl_crystal_density_diffrn    1.672
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1464
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.02
_refine_diff_density_max         0.887
_refine_diff_density_min         -0.516
_refine_diff_density_rms         0.112
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.934
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     201
_refine_ls_number_reflns         3362
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.934
_refine_ls_R_factor_all          0.1332
_refine_ls_R_factor_gt           0.0637
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0601P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1186
_refine_ls_wR_factor_ref         0.1384
_reflns_number_gt                1880
_reflns_number_total             3362
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic901219f_si_002_3.cif
_cod_data_source_block           '[2]'
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'multi scan' changed
to 'multi-scan' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        2845.6(9)
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4303670
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mn1 Mn 0.11302(6) 0.06509(3) 0.40588(8) 0.0262(2) Uani 1 1 d . . .
Mn2 Mn 0.08874(8) 0.0000 0.67044(11) 0.0239(3) Uani 1 2 d S . .
N1 N 0.4161(4) 0.0969(2) 0.3171(6) 0.0606(16) Uani 1 1 d . . .
H1 H 0.4094 0.0736 0.2484 0.073 Uiso 1 1 calc R . .
H2 H 0.4771 0.1167 0.3475 0.073 Uiso 1 1 calc R . .
N2 N 0.3524(4) 0.13933(19) 0.4817(5) 0.0430(12) Uani 1 1 d . . .
N3 N 0.2999(4) 0.19575(18) 0.6331(5) 0.0466(13) Uani 1 1 d . . .
N4 N 0.2259(5) 0.2120(2) 0.7043(7) 0.0681(17) Uani 1 1 d . . .
N5 N 0.2398(3) 0.07222(17) 0.3299(5) 0.0320(10) Uani 1 1 d . . .
H3 H 0.2349 0.0527 0.2542 0.038 Uiso 1 1 calc R . .
N6 N 0.1758(3) 0.12720(15) 0.5255(5) 0.0320(10) Uani 1 1 d . . .
H4 H 0.1346 0.1405 0.5748 0.038 Uiso 1 1 calc R . .
C1 C 0.3321(4) 0.1023(2) 0.3762(6) 0.0361(13) Uani 1 1 d . . .
C2 C 0.2733(5) 0.1512(2) 0.5400(6) 0.0361(13) Uani 1 1 d . . .
C3 C 0.3891(6) 0.2307(3) 0.6572(8) 0.067(2) Uani 1 1 d . . .
H5 H 0.4496 0.2282 0.6185 0.081 Uiso 1 1 calc R . .
C4 C 0.3747(8) 0.2694(3) 0.7468(8) 0.083(3) Uani 1 1 d . . .
H6 H 0.4227 0.2988 0.7836 0.100 Uiso 1 1 calc R . .
C5 C 0.2712(8) 0.2560(3) 0.7733(9) 0.089(3) Uani 1 1 d . . .
H7 H 0.2393 0.2761 0.8325 0.107 Uiso 1 1 calc R . .
O1 O -0.0087(3) 0.11145(14) 0.2349(4) 0.0456(11) Uani 1 1 d . . .
O2 O -0.1601(3) 0.05751(15) 0.1789(4) 0.0416(10) Uani 1 1 d . . .
C6 C -0.1068(5) 0.0987(2) 0.1578(6) 0.0392(14) Uani 1 1 d . . .
C7 C -0.1633(5) 0.1335(2) 0.0310(7) 0.0528(17) Uani 1 1 d . . .
H8 H -0.1405 0.1705 0.0545 0.079 Uiso 1 1 calc R . .
H9 H -0.2456 0.1306 0.0071 0.079 Uiso 1 1 calc R . .
H10 H -0.1408 0.1222 -0.0511 0.079 Uiso 1 1 calc R . .
O3 O 0.2042(3) 0.0000 0.5797(5) 0.0244(11) Uani 1 2 d S . .
C8 C 0.3225(6) 0.0000 0.6582(9) 0.043(2) Uani 1 2 d S . .
H11 H 0.3662 0.0000 0.5913 0.064 Uiso 1 2 calc SR . .
H12 H 0.3412 -0.0318 0.7186 0.064 Uiso 0.50 1 calc PR . .
H13 H 0.3412 0.0318 0.7186 0.064 Uiso 0.50 1 calc PR . .
O4 O 0.0563(4) 0.0000 0.2980(5) 0.0230(10) Uani 1 2 d S . .
O5 O 0.0000 0.05395(18) 0.5000 0.0400(14) Uani 1 2 d S . .
O6 O 0.475(4) 0.0731(8) 0.035(3) 0.225(17) Uani 0.50 1 d P . .
C9 C 0.5000 0.1294(8) 0.0000 0.173(8) Uani 1 2 d S . .
O7 O 0.3322(9) 0.0000 0.0857(10) 0.153(4) Uani 1 2 d S . .
O8 O 0.0845(15) 0.0000 0.044(2) 0.278(10) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Mn1 O4 86.95(17) . . ?
O5 Mn1 N5 173.33(14) . . ?
O4 Mn1 N5 93.73(18) . . ?
O5 Mn1 N6 92.28(17) . . ?
O4 Mn1 N6 175.97(17) . . ?
N5 Mn1 N6 86.58(18) . . ?
O5 Mn1 O1 90.76(13) . . ?
O4 Mn1 O1 89.15(15) . . ?
N5 Mn1 O1 95.88(17) . . ?
N6 Mn1 O1 94.82(16) . . ?
O5 Mn1 O3 79.06(14) . . ?
O4 Mn1 O3 79.80(13) . . ?
N5 Mn1 O3 94.52(16) . . ?
N6 Mn1 O3 96.16(14) . . ?
O1 Mn1 O3 165.28(13) . . ?
O5 Mn1 Mn2 48.55(9) . 5_556 ?
O4 Mn1 Mn2 41.54(13) . 5_556 ?
N5 Mn1 Mn2 133.82(13) . 5_556 ?
N6 Mn1 Mn2 138.95(13) . 5_556 ?
O1 Mn1 Mn2 76.73(10) . 5_556 ?
O3 Mn1 Mn2 88.56(9) . 5_556 ?
O5 Mn1 Mn2 42.14(8) . . ?
O4 Mn1 Mn2 84.38(12) . . ?
N5 Mn1 Mn2 131.30(13) . . ?
N6 Mn1 Mn2 92.39(13) . . ?
O1 Mn1 Mn2 132.62(11) . . ?
O3 Mn1 Mn2 37.13(11) . . ?
Mn2 Mn1 Mn2 67.63(4) 5_556 . ?
O3 Mn2 O4 162.62(19) . 5_556 ?
O3 Mn2 O2 96.85(15) . 2_556 ?
O4 Mn2 O2 95.50(14) 5_556 2_556 ?
O3 Mn2 O2 96.85(14) . 5_556 ?
O4 Mn2 O2 95.50(14) 5_556 5_556 ?
O2 Mn2 O2 89.2(2) 2_556 5_556 ?
O3 Mn2 O5 85.02(11) . 5_556 ?
O4 Mn2 O5 81.44(11) 5_556 5_556 ?
O2 Mn2 O5 173.67(13) 2_556 5_556 ?
O2 Mn2 O5 96.64(14) 5_556 5_556 ?
O3 Mn2 O5 85.02(11) . . ?
O4 Mn2 O5 81.44(11) 5_556 . ?
O2 Mn2 O5 96.64(14) 2_556 . ?
O2 Mn2 O5 173.67(13) 5_556 . ?
O5 Mn2 O5 77.47(19) 5_556 . ?
O3 Mn2 Mn1 126.69(10) . 5_556 ?
O4 Mn2 Mn1 42.27(7) 5_556 5_556 ?
O2 Mn2 Mn1 136.46(12) 2_556 5_556 ?
O2 Mn2 Mn1 86.01(10) 5_556 5_556 ?
O5 Mn2 Mn1 42.04(3) 5_556 5_556 ?
O5 Mn2 Mn1 88.02(8) . 5_556 ?
O3 Mn2 Mn1 126.69(10) . 2_556 ?
O4 Mn2 Mn1 42.27(7) 5_556 2_556 ?
O2 Mn2 Mn1 86.01(10) 2_556 2_556 ?
O2 Mn2 Mn1 136.46(12) 5_556 2_556 ?
O5 Mn2 Mn1 88.02(8) 5_556 2_556 ?
O5 Mn2 Mn1 42.04(3) . 2_556 ?
Mn1 Mn2 Mn1 68.93(4) 5_556 2_556 ?
O3 Mn2 Mn1 48.43(9) . 6 ?
O4 Mn2 Mn1 118.12(11) 5_556 6 ?
O2 Mn2 Mn1 145.27(12) 2_556 6 ?
O2 Mn2 Mn1 95.59(11) 5_556 6 ?
O5 Mn2 Mn1 36.83(2) 5_556 6 ?
O5 Mn2 Mn1 81.10(8) . 6 ?
Mn1 Mn2 Mn1 78.27(3) 5_556 6 ?
Mn1 Mn2 Mn1 112.37(4) 2_556 6 ?
O3 Mn2 Mn1 48.43(9) . . ?
O4 Mn2 Mn1 118.12(11) 5_556 . ?
O2 Mn2 Mn1 95.59(11) 2_556 . ?
O2 Mn2 Mn1 145.27(12) 5_556 . ?
O5 Mn2 Mn1 81.10(8) 5_556 . ?
O5 Mn2 Mn1 36.83(2) . . ?
Mn1 Mn2 Mn1 112.37(4) 5_556 . ?
Mn1 Mn2 Mn1 78.27(3) 2_556 . ?
Mn1 Mn2 Mn1 62.13(4) 6 . ?
C2 N2 C1 120.3(4) . . ?
C3 N3 N4 110.9(5) . . ?
C3 N3 C2 128.7(6) . . ?
N4 N3 C2 120.2(5) . . ?
C5 N4 N3 105.1(6) . . ?
C1 N5 Mn1 129.4(4) . . ?
C2 N6 Mn1 127.3(4) . . ?
N5 C1 N1 119.8(5) . . ?
N5 C1 N2 125.7(5) . . ?
N1 C1 N2 114.5(5) . . ?
N2 C2 N6 129.4(5) . . ?
N2 C2 N3 114.0(5) . . ?
N6 C2 N3 116.6(5) . . ?
C4 C3 N3 107.5(7) . . ?
C3 C4 C5 105.2(6) . . ?
N4 C5 C4 111.2(7) . . ?
C6 O1 Mn1 128.7(4) . . ?
C6 O2 Mn2 123.8(3) . 5_556 ?
O1 C6 O2 124.2(5) . . ?
O1 C6 C7 117.4(5) . . ?
O2 C6 C7 118.4(5) . . ?
C8 O3 Mn2 123.0(4) . . ?
C8 O3 Mn1 124.3(3) . 6 ?
Mn2 O3 Mn1 94.43(14) . 6 ?
C8 O3 Mn1 124.3(3) . . ?
Mn2 O3 Mn1 94.43(14) . . ?
Mn1 O3 Mn1 86.89(15) 6 . ?
Mn2 O4 Mn1 96.19(15) 5_556 . ?
Mn2 O4 Mn1 96.19(15) 5_556 6 ?
Mn1 O4 Mn1 113.5(2) . 6 ?
Mn1 O5 Mn1 163.4(3) . 2_556 ?
Mn1 O5 Mn2 89.41(8) . 5_556 ?
Mn1 O5 Mn2 101.03(9) 2_556 5_556 ?
Mn1 O5 Mn2 101.03(9) . . ?
Mn1 O5 Mn2 89.41(8) 2_556 . ?
Mn2 O5 Mn2 102.53(19) 5_556 . ?
O6 O6 C9 69.5(11) 2_655 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mn1 O5 1.9190(10) . ?
Mn1 O4 1.939(2) . ?
Mn1 N5 1.941(4) . ?
Mn1 N6 1.944(4) . ?
Mn1 O1 2.187(4) . ?
Mn1 O3 2.358(3) . ?
Mn1 Mn2 2.8655(11) 5_556 ?
Mn1 Mn2 3.1423(13) . ?
Mn2 O3 1.903(4) . ?
Mn2 O4 1.911(4) 5_556 ?
Mn2 O2 2.041(4) 2_556 ?
Mn2 O2 2.041(4) 5_556 ?
Mn2 O5 2.148(3) 5_556 ?
Mn2 O5 2.148(3) . ?
Mn2 Mn1 2.8655(11) 5_556 ?
Mn2 Mn1 2.8655(11) 2_556 ?
Mn2 Mn1 3.1423(13) 6 ?
N1 C1 1.345(7) . ?
N2 C2 1.311(7) . ?
N2 C1 1.345(7) . ?
N3 C3 1.364(7) . ?
N3 N4 1.372(7) . ?
N3 C2 1.405(7) . ?
N4 C5 1.316(8) . ?
N5 C1 1.318(6) . ?
N6 C2 1.311(6) . ?
C3 C4 1.351(10) . ?
C4 C5 1.421(11) . ?
O1 C6 1.247(6) . ?
O2 C6 1.270(6) . ?
O2 Mn2 2.041(4) 5_556 ?
C6 C7 1.491(8) . ?
O3 C8 1.418(7) . ?
O3 Mn1 2.358(3) 6 ?
O4 Mn2 1.911(4) 5_556 ?
O4 Mn1 1.939(2) 6 ?
O5 Mn1 1.9190(10) 2_556 ?
O5 Mn2 2.148(3) 5_556 ?
O6 O6 1.05(6) 2_655 ?
O6 C9 1.50(2) . ?
C9 O6 1.50(2) 2_655 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O5 Mn1 Mn2 O3 172.2(2) . . . . ?
O4 Mn1 Mn2 O3 80.52(17) . . . . ?
N5 Mn1 Mn2 O3 -9.5(2) . . . . ?
N6 Mn1 Mn2 O3 -97.06(17) . . . . ?
O1 Mn1 Mn2 O3 164.16(19) . . . . ?
Mn2 Mn1 Mn2 O3 119.91(12) 5_556 . . . ?
O5 Mn1 Mn2 O4 5.68(18) . . . 5_556 ?
O4 Mn1 Mn2 O4 -85.97(13) . . . 5_556 ?
N5 Mn1 Mn2 O4 -176.00(19) . . . 5_556 ?
N6 Mn1 Mn2 O4 96.45(15) . . . 5_556 ?
O1 Mn1 Mn2 O4 -2.33(17) . . . 5_556 ?
O3 Mn1 Mn2 O4 -166.49(15) . . . 5_556 ?
Mn2 Mn1 Mn2 O4 -46.59(9) 5_556 . . 5_556 ?
O5 Mn1 Mn2 O2 -93.61(19) . . . 2_556 ?
O4 Mn1 Mn2 O2 174.73(16) . . . 2_556 ?
N5 Mn1 Mn2 O2 84.70(19) . . . 2_556 ?
N6 Mn1 Mn2 O2 -2.85(16) . . . 2_556 ?
O1 Mn1 Mn2 O2 -101.63(18) . . . 2_556 ?
O3 Mn1 Mn2 O2 94.21(16) . . . 2_556 ?
Mn2 Mn1 Mn2 O2 -145.88(11) 5_556 . . 2_556 ?
O5 Mn1 Mn2 O2 169.8(2) . . . 5_556 ?
O4 Mn1 Mn2 O2 78.1(2) . . . 5_556 ?
N5 Mn1 Mn2 O2 -11.9(3) . . . 5_556 ?
N6 Mn1 Mn2 O2 -99.5(2) . . . 5_556 ?
O1 Mn1 Mn2 O2 161.8(2) . . . 5_556 ?
O3 Mn1 Mn2 O2 -2.4(2) . . . 5_556 ?
Mn2 Mn1 Mn2 O2 117.50(18) 5_556 . . 5_556 ?
O5 Mn1 Mn2 O5 80.9(2) . . . 5_556 ?
O4 Mn1 Mn2 O5 -10.71(13) . . . 5_556 ?
N5 Mn1 Mn2 O5 -100.74(18) . . . 5_556 ?
N6 Mn1 Mn2 O5 171.71(14) . . . 5_556 ?
O1 Mn1 Mn2 O5 72.93(16) . . . 5_556 ?
O3 Mn1 Mn2 O5 -91.23(13) . . . 5_556 ?
Mn2 Mn1 Mn2 O5 28.68(6) 5_556 . . 5_556 ?
O4 Mn1 Mn2 O5 -91.7(2) . . . . ?
N5 Mn1 Mn2 O5 178.3(2) . . . . ?
N6 Mn1 Mn2 O5 90.8(2) . . . . ?
O1 Mn1 Mn2 O5 -8.0(2) . . . . ?
O3 Mn1 Mn2 O5 -172.2(2) . . . . ?
Mn2 Mn1 Mn2 O5 -52.27(16) 5_556 . . . ?
O5 Mn1 Mn2 Mn1 52.27(16) . . . 5_556 ?
O4 Mn1 Mn2 Mn1 -39.39(12) . . . 5_556 ?
N5 Mn1 Mn2 Mn1 -129.42(17) . . . 5_556 ?
N6 Mn1 Mn2 Mn1 143.03(13) . . . 5_556 ?
O1 Mn1 Mn2 Mn1 44.26(14) . . . 5_556 ?
O3 Mn1 Mn2 Mn1 -119.91(12) . . . 5_556 ?
Mn2 Mn1 Mn2 Mn1 0.0 5_556 . . 5_556 ?
O5 Mn1 Mn2 Mn1 -8.87(16) . . . 2_556 ?
O4 Mn1 Mn2 Mn1 -100.53(13) . . . 2_556 ?
N5 Mn1 Mn2 Mn1 169.44(17) . . . 2_556 ?
N6 Mn1 Mn2 Mn1 81.89(12) . . . 2_556 ?
O1 Mn1 Mn2 Mn1 -16.89(15) . . . 2_556 ?
O3 Mn1 Mn2 Mn1 178.95(12) . . . 2_556 ?
Mn2 Mn1 Mn2 Mn1 -61.14(3) 5_556 . . 2_556 ?
O5 Mn1 Mn2 Mn1 114.47(16) . . . 6 ?
O4 Mn1 Mn2 Mn1 22.81(12) . . . 6 ?
N5 Mn1 Mn2 Mn1 -67.22(17) . . . 6 ?
N6 Mn1 Mn2 Mn1 -154.77(12) . . . 6 ?
O1 Mn1 Mn2 Mn1 106.45(14) . . . 6 ?
O3 Mn1 Mn2 Mn1 -57.71(12) . . . 6 ?
Mn2 Mn1 Mn2 Mn1 62.20(2) 5_556 . . 6 ?
C3 N3 N4 C5 -1.1(8) . . . . ?
C2 N3 N4 C5 -175.8(6) . . . . ?
O4 Mn1 N5 C1 -164.9(4) . . . . ?
N6 Mn1 N5 C1 11.1(5) . . . . ?
O1 Mn1 N5 C1 105.6(5) . . . . ?
O3 Mn1 N5 C1 -84.8(5) . . . . ?
Mn2 Mn1 N5 C1 -177.2(4) 5_556 . . . ?
Mn2 Mn1 N5 C1 -79.1(5) . . . . ?
O5 Mn1 N6 C2 166.3(4) . . . . ?
N5 Mn1 N6 C2 -7.2(4) . . . . ?
O1 Mn1 N6 C2 -102.8(4) . . . . ?
O3 Mn1 N6 C2 87.0(4) . . . . ?
Mn2 Mn1 N6 C2 -178.1(3) 5_556 . . . ?
Mn2 Mn1 N6 C2 124.1(4) . . . . ?
Mn1 N5 C1 N1 172.7(4) . . . . ?
Mn1 N5 C1 N2 -7.0(8) . . . . ?
C2 N2 C1 N5 -5.6(9) . . . . ?
C2 N2 C1 N1 174.7(5) . . . . ?
C1 N2 C2 N6 10.1(9) . . . . ?
C1 N2 C2 N3 -171.2(5) . . . . ?
Mn1 N6 C2 N2 -1.5(8) . . . . ?
Mn1 N6 C2 N3 179.8(3) . . . . ?
C3 N3 C2 N2 7.9(9) . . . . ?
N4 N3 C2 N2 -178.5(5) . . . . ?
C3 N3 C2 N6 -173.3(6) . . . . ?
N4 N3 C2 N6 0.4(8) . . . . ?
N4 N3 C3 C4 1.1(8) . . . . ?
C2 N3 C3 C4 175.3(6) . . . . ?
N3 C3 C4 C5 -0.7(9) . . . . ?
N3 N4 C5 C4 0.6(9) . . . . ?
C3 C4 C5 N4 0.1(10) . . . . ?
O5 Mn1 O1 C6 -52.8(5) . . . . ?
O4 Mn1 O1 C6 34.1(5) . . . . ?
N5 Mn1 O1 C6 127.8(5) . . . . ?
N6 Mn1 O1 C6 -145.2(5) . . . . ?
O3 Mn1 O1 C6 -7.0(10) . . . . ?
Mn2 Mn1 O1 C6 -5.9(5) 5_556 . . . ?
Mn2 Mn1 O1 C6 -47.5(6) . . . . ?
Mn1 O1 C6 O2 9.6(9) . . . . ?
Mn1 O1 C6 C7 -168.9(4) . . . . ?
Mn2 O2 C6 O1 -7.0(8) 5_556 . . . ?
Mn2 O2 C6 C7 171.5(4) 5_556 . . . ?
O4 Mn2 O3 C8 180.000(2) 5_556 . . . ?
O2 Mn2 O3 C8 44.99(10) 2_556 . . . ?
O2 Mn2 O3 C8 -44.99(10) 5_556 . . . ?
O5 Mn2 O3 C8 -141.09(9) 5_556 . . . ?
O5 Mn2 O3 C8 141.09(9) . . . . ?
Mn1 Mn2 O3 C8 -135.11(8) 5_556 . . . ?
Mn1 Mn2 O3 C8 135.11(8) 2_556 . . . ?
Mn1 Mn2 O3 C8 -136.39(8) 6 . . . ?
Mn1 Mn2 O3 C8 136.39(8) . . . . ?
O4 Mn2 O3 Mn1 -43.61(8) 5_556 . . 6 ?
O2 Mn2 O3 Mn1 -178.62(12) 2_556 . . 6 ?
O2 Mn2 O3 Mn1 91.41(13) 5_556 . . 6 ?
O5 Mn2 O3 Mn1 -4.70(12) 5_556 . . 6 ?
O5 Mn2 O3 Mn1 -82.51(13) . . . 6 ?
Mn1 Mn2 O3 Mn1 1.28(15) 5_556 . . 6 ?
Mn1 Mn2 O3 Mn1 -88.49(4) 2_556 . . 6 ?
Mn1 Mn2 O3 Mn1 -87.21(16) . . . 6 ?
O4 Mn2 O3 Mn1 43.61(8) 5_556 . . . ?
O2 Mn2 O3 Mn1 -91.41(13) 2_556 . . . ?
O2 Mn2 O3 Mn1 178.62(12) 5_556 . . . ?
O5 Mn2 O3 Mn1 82.51(13) 5_556 . . . ?
O5 Mn2 O3 Mn1 4.70(12) . . . . ?
Mn1 Mn2 O3 Mn1 88.49(4) 5_556 . . . ?
Mn1 Mn2 O3 Mn1 -1.28(15) 2_556 . . . ?
Mn1 Mn2 O3 Mn1 87.21(16) 6 . . . ?
O5 Mn1 O3 C8 -140.9(5) . . . . ?
O4 Mn1 O3 C8 130.3(5) . . . . ?
N5 Mn1 O3 C8 37.3(5) . . . . ?
N6 Mn1 O3 C8 -49.8(5) . . . . ?
O1 Mn1 O3 C8 172.2(6) . . . . ?
Mn2 Mn1 O3 C8 171.1(4) 5_556 . . . ?
Mn2 Mn1 O3 C8 -135.6(5) . . . . ?
O5 Mn1 O3 Mn2 -5.34(13) . . . . ?
O4 Mn1 O3 Mn2 -94.17(17) . . . . ?
N5 Mn1 O3 Mn2 172.85(16) . . . . ?
N6 Mn1 O3 Mn2 85.81(16) . . . . ?
O1 Mn1 O3 Mn2 -52.2(6) . . . . ?
Mn2 Mn1 O3 Mn2 -53.31(10) 5_556 . . . ?
O5 Mn1 O3 Mn1 88.87(14) . . . 6 ?
O4 Mn1 O3 Mn1 0.04(16) . . . 6 ?
N5 Mn1 O3 Mn1 -92.95(16) . . . 6 ?
N6 Mn1 O3 Mn1 -179.99(16) . . . 6 ?
O1 Mn1 O3 Mn1 42.0(7) . . . 6 ?
Mn2 Mn1 O3 Mn1 40.90(10) 5_556 . . 6 ?
Mn2 Mn1 O3 Mn1 94.21(14) . . . 6 ?
O5 Mn1 O4 Mn2 20.05(14) . . . 5_556 ?
N5 Mn1 O4 Mn2 -166.60(16) . . . 5_556 ?
O1 Mn1 O4 Mn2 -70.76(16) . . . 5_556 ?
O3 Mn1 O4 Mn2 99.47(17) . . . 5_556 ?
Mn2 Mn1 O4 Mn2 62.24(12) . . . 5_556 ?
O5 Mn1 O4 Mn1 -79.5(2) . . . 6 ?
N5 Mn1 O4 Mn1 93.9(2) . . . 6 ?
O1 Mn1 O4 Mn1 -170.3(2) . . . 6 ?
O3 Mn1 O4 Mn1 0.0(2) . . . 6 ?
Mn2 Mn1 O4 Mn1 -99.5(3) 5_556 . . 6 ?
Mn2 Mn1 O4 Mn1 -37.28(19) . . . 6 ?
O4 Mn1 O5 Mn1 -146.99(11) . . . 2_556 ?
N6 Mn1 O5 Mn1 36.97(12) . . . 2_556 ?
O1 Mn1 O5 Mn1 -57.88(10) . . . 2_556 ?
O3 Mn1 O5 Mn1 132.81(8) . . . 2_556 ?
Mn2 Mn1 O5 Mn1 -129.34(9) 5_556 . . 2_556 ?
Mn2 Mn1 O5 Mn1 128.01(12) . . . 2_556 ?
O4 Mn1 O5 Mn2 -17.65(14) . . . 5_556 ?
N6 Mn1 O5 Mn2 166.31(15) . . . 5_556 ?
O1 Mn1 O5 Mn2 71.46(14) . . . 5_556 ?
O3 Mn1 O5 Mn2 -97.85(13) . . . 5_556 ?
Mn2 Mn1 O5 Mn2 -102.7(2) . . . 5_556 ?
O4 Mn1 O5 Mn2 85.00(16) . . . . ?
N6 Mn1 O5 Mn2 -91.04(17) . . . . ?
O1 Mn1 O5 Mn2 174.11(15) . . . . ?
O3 Mn1 O5 Mn2 4.80(12) . . . . ?
Mn2 Mn1 O5 Mn2 102.7(2) 5_556 . . . ?
O3 Mn2 O5 Mn1 -5.87(14) . . . . ?
O4 Mn2 O5 Mn1 -174.93(16) 5_556 . . . ?
O2 Mn2 O5 Mn1 90.47(17) 2_556 . . . ?
O5 Mn2 O5 Mn1 -91.86(13) 5_556 . . . ?
Mn1 Mn2 O5 Mn1 -132.96(13) 5_556 . . . ?
Mn1 Mn2 O5 Mn1 167.0(2) 2_556 . . . ?
Mn1 Mn2 O5 Mn1 -54.53(12) 6 . . . ?
O3 Mn2 O5 Mn1 -172.84(14) . . . 2_556 ?
O4 Mn2 O5 Mn1 18.10(12) 5_556 . . 2_556 ?
O2 Mn2 O5 Mn1 -76.50(15) 2_556 . . 2_556 ?
O5 Mn2 O5 Mn1 101.17(11) 5_556 . . 2_556 ?
Mn1 Mn2 O5 Mn1 60.07(11) 5_556 . . 2_556 ?
Mn1 Mn2 O5 Mn1 138.50(11) 6 . . 2_556 ?
Mn1 Mn2 O5 Mn1 -167.0(2) . . . 2_556 ?
O3 Mn2 O5 Mn2 86.00(8) . . . 5_556 ?
O4 Mn2 O5 Mn2 -83.07(9) 5_556 . . 5_556 ?
O2 Mn2 O5 Mn2 -177.66(12) 2_556 . . 5_556 ?
O5 Mn2 O5 Mn2 0.0 5_556 . . 5_556 ?
Mn1 Mn2 O5 Mn2 -41.099(19) 5_556 . . 5_556 ?
Mn1 Mn2 O5 Mn2 -101.17(11) 2_556 . . 5_556 ?
Mn1 Mn2 O5 Mn2 37.33(2) 6 . . 5_556 ?
Mn1 Mn2 O5 Mn2 91.86(13) . . . 5_556 ?
